- Email: [email protected]

Thermal transport in SiC nanostructures E. Ziambaras *, P. Hyldgaard Department of Applied Physics, Chalmers University of Technology and Go¨teborg University, SE-412 96 Go¨teborg, Sweden Available online 8 August 2005

Abstract SiC is a robust semiconductor material considered ideal for high-power application due to its material stability and large bulk thermal conductivity defined by the very fast phonons In this paper, however, we show that both material-interface scattering and total internal reflection significantly limit the SiC-nanostructure phonon transport and hence the heat dissipation in a typical device. For simplicity we focus on planar SiC nanostructures and calculate the thermal transport both parallel to the layers in a substrate/SiC/oxide heterostructure and across a SiC/metal gate or contact. We find that the phonon-interface scattering produces a heterostructure thermal conductivity significantly smaller than what is predicted in a traditional heat transport calculation. We also document that the high temperature heat flow across the metal/SiC interface is limited by total internal reflection effects and maximizes with a small difference in the metal/SiC sound velocities. D 2005 Elsevier B.V. All rights reserved. Keywords: Phonon thermal transport; SiC nanostructure devices; Knudsen effect

1. Introduction SiC is an exciting material with possible application in high-power devices but also posing interesting challenges for our understanding of the necessary heat dissipation. There are several SiC advantages, for example, structural robustness, presence of a native oxide (SiO2), durability, and ability to grow high-mobility SiC layers on top of cheap Si substrates. The set of very fast phonons, the high purity, and the long phonon mean free path l mfp also ensures a very large bulk thermal conductivity. On the one hand this raises the promise for high-power device applications since it indicates effective heat dissipation. On the other hand, the micron scale l mfp invalidates the foundation of the traditional analysis based on the Fourier law of thermal transport. A finite-element approach that describes the local flow in terms of bulk values for the thermal conductivities breaks down because the phonon mean free path now approaches or exceeds typical feature sizes (thickness of conduction channel and oxide layers and distance between gates and

* Corresponding author. Tel.: +46 31 772 8427; fax: +46 31 772 8426. E-mail address: [email protected] (E. Ziambaras). 0928-4931/$ - see front matter D 2005 Elsevier B.V. All rights reserved. doi:10.1016/j.msec.2005.06.044

contacts). We must instead turn to phonon-based calculations to describe SiC devices that represent a natural test case for developing an understanding of nanostructure thermal transport [1]. Fig. 1 shows a structural schematics (upper panel) of a SiC device for which we document two phonon transport effects (lower panels) that significantly suppresses the heat dissipation. We observe that the thermal transport is completely dominated by the phonon dynamics even when discussing the conductance across a SiC/metal interface. For the phonon transmission problem we calculate the thermal conductance of SiC interfaces at room temperature, h = 300 K, and report the variation with general ratios of the material acoustic impedances and sound velocities. We find that this thermal conductance exhibits only a weak dependence on the ratio of acoustic impedances (which determines the long-wavelength phonon transmission) but a strong variation with the ratio of the material sound velocities (that define the total internal reflection of phonons). In contrast to what is normally assumed we argue that heat dissipation can be maximized by matching the sound velocities of the SiC and metal (or substrate). We also document a phonon Knudsen effect that causes a significant suppression of the in-plane thermal conductivity

636

E. Ziambaras, P. Hyldgaard / Materials Science and Engineering C 25 (2005) 635 – 640

based description of thermal dissipation will become increasingly important with a continued downscaling.

2. Suppression of thermal transport across SiC/metal interfaces Fig. 2 illustrates the atomistic simple-cubic (SC) model adapted to estimate the finite-temperature thermal transport across the SiC/metal (or SiC/Si-substrate) inter face. Both the phonon frequency x and the in-plane momentum q|| (parallel to the interface) is conserved in this description of the phonon transmission. While approximative, our model description retains the important transport consequences of phonon total internal reflection [2,3]. This SC atomistic model has previously been used to calculate the phonon transmission and thermal transport in Si/Ge superlattices and heterostructures [2,3]. Here we extend the SC model to describe the binary nature of the SiC material by choosing the SC volume a sc3 to contain exactly one physical atom but having an average atomic ˚ mass M SiC = (M Si + M C) / 2. The value of a sc = 2.18 A corresponds to the physical (FCC) lattice constant ˚ of SiC [4]. Within each of the materials, these a 0 = 4.36 A SC volumes are linked by force constants F p,t;SiC with values which are fitted to pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ the SiC sound velocities [4] cl;t;SiC ¼ asc Fp;t;SiC =MSiC , as expressed in the SC approximation [2]. In this model we also obtain acoustic pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ impedances [3] Zl;t;SiC ¼ Fp;t;SiC MSiC =a2sc . We use a corresponding notation ( F p,t;me, M me, . . .) to describe the SC phonon dynamics in the neighboring media Fme_ (metal, Si, or general substrate). We assume for simplicity an identical lattice constant a sc for both the SiC and the

Fig. 1. Structural schematics (top panel) and summary of key phonon transport effects (bottom panels) in a typical nanoscale SiC device. Oxide and substrate layers together with SiC/metal interfaces surround the thin (undoped) SiC transport channel. We find that heat dissipation is suppressed at room temperatures by the ineffective phonon transmission FT_ (lower left panel) across the SiC/metal or SiC/Si interfaces and by the phonon Knudsen effect FK_ (lower right panel), that is, the suppression of the thermal conductivity within the SiC by interface scattering at layer thicknesses d layer < 5 Am. The phonon transport is calculated analytically at general probabilities, p +() and 1 p +(), for specular and diffusive scattering at the upper (lower) interface.

for nanoscale layer thicknesses at room temperatures and even microscale thicknesses at liquid-nitrogen temperatures, h å 77 K. At the same time we show that the traditional Fourier analysis breaks down in the description of such small structures and stress that shifting toward a phononθ MSiC

Kp

Fp,SiC

Fp,me

a sc

k

Mme

a sc

Silicon carbide

me: Metal or substrate

Ft,SiC

q

Ft,me

Fp,SiC Ft,SiC

Fp,me Fp,me

Fp,SiC Ft,me

Fig. 2. Schematics of the effective, atomistic representation in a simple-cubic (SC) model [2] adapted to estimate the finite-temperature phonon transport across SiC/metal (and SiC/Si) interface (vertical dashed line). The SC volume a sc3 is chosen to contain exactly one physical atom but having the average atomic mass M SiC = (M Si + M C) / 2. A similar approach describes the neighboring media Fme_ (metal or Si substrate). Force constants, F p,t;SiC (me) fittedﬃ to the longitudinal pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ and transverse sound velocities [2,3], link the SC volumes within the SiC (metal) while elastic coupling constants Kp;t u Fp;t;SiC Fp;t;me connect across the interface [3].

E. Ziambaras, P. Hyldgaard / Materials Science and Engineering C 25 (2005) 635 – 640

adjacent material and we approximate the ﬃelastic coupling pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ across the interface by Kp;t u Fp;t;SiC Fp;t;me. Our calculation of the phonon conductance r K across the SiC/metal or SiC/substrate interface follows the approach and analysis of Ref. [3] to which we refer for a more detailed discussion. The modes in our SC model can be polarized either parallel (Fp_) or at right angles (Ft_) to the interface normal. In the following we focus on the description of the phonon dynamics and transmission of Fp_-polarized modes. The dynamics of a phonon moving in the SiC or neighboring media Fme_ is then unique characterized by the conserved set (x, q ||). Weﬃ introduce pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ frequencies Xp;t;SiCðmeÞ ¼ 2 Fp;t;SiCðmeÞ =MSiCðmeÞ and the (conserved) dimensionless measure a q|| = 2 cos( q x a sc) cos( q y a sc) of the in-plane-dynamics. The SC phonon dispersion relation can be expressed as X2p;SiCðmeÞ 1 cos kSiCðmeÞ asc ¼ 2x2 X2t;SiCðmeÞ aq

637

too much energy to enter the (softer) metal or substrate. In our SC model, both of these situations cause the dispersion relation (1) to yield an imaginary value of kSiC (me), i.e., the correct attenuated behavior on the SiC(me) side of the interface. At elevated temperatures and with a finite separation in the sound velocities (material hardness) such total-internal reflection suppresses the thermal transport contribution from most of the available phase space [2,3]. To quantify the resulting suppression of the conductance we calculate the SC estimates for the probability T K(x, q ||) of phonon tunneling at general x and q || within our SC model. We extract T K(x, q ||) by solving the Newton equation of motion for the phonon displacement g q||;SiC(l 0) and g q||;me(s 1) of the (atom scale) SC elements located at the interface (here located between l = 0 and s = 1). Specifically, we consider then the reflection and transmission of an incoming SiC mode

ð1Þ and serves to establish the perpendicular momentum component kSiC(me) of any phonon mode (x, q ||) when moving in the SiC (and/or in the metal or substrate Fme_). We emphasize that this SC model description includes the effects of attenuation and of phonon total-internal reflection. The attenuation (with associated thermal transport suppression) arises because there is either insufficient or excess energy available for the perpendicular dynamics. A phonon with in-plane momentum q || > 0 that approaches from the typically softer Fme_ side can be blocked from entering the hard SiC because the mode have too little energy to sustain the in-plane dynamics. Conversely a mode (x, q ||) which propagates in the SiC (having a real value of kSiC) can have

gq ;SiC ðlV0Þ ¼ eikSiC asc l þ AeikSiC asc l

ð2Þ

gq ;me ðsz1Þ ¼ Beikme asc s ;

ð3Þ

and solve the harmonic equation gq ;me ðs ¼ 1Þ x2 X2t;me aq =2 ¼

i Fp;me h gq ;me ðs ¼ 2Þ gq ;me ðs ¼ 1Þ Mme i Kp h þ gq ; me ðs ¼ 1Þ gq ;SiC ðl ¼ 0Þ : Mme

ð4Þ

The tunneling vanishes of course exactly when there is attenuation on either side of the interface. In the case when

3

σκ [W/m2K] 105

2.5

300 K

2 1.5 1 0.5 0 2 2

1.5 1.5

1

c me /c SiC

1

0.5

0.5 0

Z me /Z SiC

0

Fig. 3. Dramatic variation of the room-temperature thermal conductance r K across a SiC/general-media interface specified by key differences in materials’ properties. A strong (weaker) dependence arises with the variation in the ratio of material sound velocities c (acoustic impedance Z) which specifies the amount of total internal phonon reflection (long-wavelength tunneling probability).

638

E. Ziambaras, P. Hyldgaard / Materials Science and Engineering C 25 (2005) 635 – 640

Table 1 Materials’ properties and model parameters for the calculation of the room-temperature thermal transport across SiC/metal and/or SiC/Si interfaces

SiC (FCC) Si (FCC) Al (FCC) Ni (FCC) Cu (FCC) Ag (FCC)

˚) a 0 (A

M (amu)

˚) a sc (A

c l (m/s)

c t (m/s)

(Z me / Z SiC)l

(Z me / Z SiC)t

(c me / c SiC)l

(c me / c SiC)t

4.36 5.43 4.05 3.52 3.61 4.09

20.05 28.09 26.99 58.71 63.55 107.87

2.188 2.715 2.551 2.218 2.274 2.576

13035 8470 6360 5810 4760 3640

6257 5340 3130 3080 2320 1690

1 0.65 0.41 1.25 1.02 0.92

1 0.85 0.42 1.38 1.04 0.89

1 0.48 0.49 0.45 0.36 0.28

1 0.63 0.50 0.49 0.37 0.27

both kSiC and kme are real, we determine the tunneling probability TK x; aq ¼ 1 jAj2 ð5Þ and hence obtain a description of the transport contribution at general (x, q ||). We calculate the finite-temperature thermal conductance across the SiC/metal interface by use of the formal result [5,3]: rK ¼

X Z d 2 q Z dx BN0 JxT ð x; q Þ : K 8 2k Bh ð2kÞ2 modes

ð6Þ

The Ffree_ interface thermal conductance r 0 that describes the phonon transmission across SiC/SiC interfaces (for example, between the doped SiC substrate and the undoped SiC transport channel) serves as a natural reference. We typically have the situation r K(h) N r 0(h) at finite temperatures [3] (for example, above the liquidnitrogen temperature). Fig. 3 shows the results for the thermal conductance, r K, calculated at h = 300 K for a general SiC/metal or SiC/ substrate interface within the SC model description. The plot reports a dramatic variation of r K as a function of the ratio of sound velocities c me / c SiC and a much weaker dependence on the ratio of acoustic impedances Z me / Z SiC. Inserting the value for these ratios from Table 1, the figure also documents that the typical SiC/metal and the SiC/Si interface at h = 300 K causes a dramatic suppression of the thermal conductance (when compared to the free conductance value given by c me / c SiC = Z me / Z SiC K 1). The study identifies the need for further improving our understanding of the thermal coupling at such interfaces. We also stress that this suppression of r K is qualitatively and quantitatively very different from the traditional conductance variation in low-temperature Kapitza effect. In the low-temperature regime the transmission is given by classical acoustics and hence exclusively defined by the ratio Z me / Z SiC. In the present finite-temperature regime it is instead the total internal phonon reflection and hence c me / c SiC that specifies the dominant thermal conductance variation. In general the contact region between SiC and metals possesses a complex structure. Our calculation of the r K variation assumes a perfect junction between the SiC and the metal or Si substrate, rests on a simplified description of

the characteristic phonon modes, and can thus only provide an approximative description. Nevertheless our results strongly indicate that it is the difference in sound velocities rather than (as often assumed) the ratio of acoustic impedances which should be matched to maximize the high-temperature thermal transport out from SiC power devices at contact gates and cooling fringes.

3. Suppression of the thermal transport in SiC layers We calculate the phonon Knudsen effect on the in-plane thermal transport by solving the linearized Boltzmann transport equation (l-BTE) in the relaxation-time approximation [6]. We consider a layer of thickness d layer in which a small thermal gradient, lh||x, induces a change yN from the equilibrium phonon distribution N 0 = 1 / (eHx / kBh 1). The upper, lower material boundaries are placed at z >,< = Td layer / 2 and we use here q z / q || to denote the component of the total phonon momentum q that is perpendicular to the layers/parallel to the in-plane temperature gradient lh, respectively.1 The bulk phonon mean free path, lmfp ¼ vq sq is given by the product of the phonon group velocity and the (bulk) relaxation time. We assume, for simplicity, that l mfp is independent of the mode and momentum and we fit l mfp against measurements of the bulk-SiC thermal conductivity [7]. Solving then the l-BTE

qz B 1 1 BN0 þ ð7Þ yN ¼ q lh ; q Bh q Bz lmfp in the absence and presence of the first term we obtain and compare the distribution changes yN bulk and ð8Þ yNlayer ¼ yNbulk 1 hqz ð z; pþ ; p Þ : These distribution changes, in turn, determine the phonon thermal conductivity X Z dq Z dqz Z dqy 1 jbulk;layer ¼ ðlhÞ ð2kÞ ð2kÞ ð2kÞ modes Jxq vq yNbulk;layer

ð9Þ

in the bulk and in the layered structure, respectively. 1 The other in-plane momentum component is denoted q y ; we seek to keep a consistent notation between the two calculations although the direction of the temperature gradient differs.

E. Ziambaras, P. Hyldgaard / Materials Science and Engineering C 25 (2005) 635 – 640

SiO2 Pure SiC

300

d SiO =100 nm 2 d layer =0–500 nm

κ eff [W/Km]

Si-substrate

639

300 K

d Sub =500 nm

200

100

0

κeff =Σ iκ (di )di/Σidi

pSiC/Si =0; Present approach pSiC/Si =1; Present approach Traditional Fourier approach 0

100

i=oxide, layer, substrate

200

300

400

500

dlayer [nm] 2000

77 K κ eff [W/Km]

1600

SiO2 Pure SiC

1200

pSiC/Si=0; Present approach pSiC/Si=1; Present approach Traditional Fourier approach

800

Si-substrate

d SiO =100 nm 2

d layer =0–1000 nm d Sub =2000 nm

400 0

0

200

400

600

800

1000

dlayer [nm] Fig. 4. Knudsen suppression of the effective in-plane SiC transport j eff by interface scattering in the typical layered structures (insets). The upper (lower) panel reports the variation with the thickness d layer of SiC conductance channel at room (liquid-nitrogen) temperatures assuming either diffusive (solid curves) or specular (dashed curves) scattering at the SiC/Si substrate interface. The traditional approach based on the Fourier law of heat flow (dotted curves) is documented to be inadequate due to the micron-scale phonon mean free path.

The interface scattering causes a suppression hqz ð z; pþ ; p Þ ¼

X

using special functions Qð j; g; p; pˆ Þ ¼ pˆ 2 2p þ 1 pˆ j1 Dð jgÞ

/nqz ðpþ ; p Þejzzn j=flmfp ðjq8 j=qÞg

þ ðp pˆ Þðpˆ þ 1Þ2 pˆ 2ð j1Þ Dð 2jgÞ

n¼>;<

ð10Þ which depends on the fraction of specular p +() and diffusive 1 p +() scattering at theupper (lower) material boundary. We determine the amplitudes / q>,< of this z variationfrom an analysis of the phonon scattering at the two interfaces z >,< = T d layer / 2,following Refs. [7 –9]. Specifically for phonons that travel toward z > = d / 2 (withperpendicular momentum q z > 0), the appropriate boundary condition for specularscattering is yN(X,q –) K yN(X, q z ) while the corresponding boundary conditionfor diffusive scattering is yN(X,q z < 0) K 0. A similar treatment yields the boundary conditions at the lower interface, z <, and an approach to determine the full variation of the suppression (Eq. (10)) by interface scattering. pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ We introduce p¯ = ( p + + p ) / 2 and pˆ ¼ pþ p and express the resulting phonon Knudsen effect jlayer 3 ðg; pþ ; p Þ ¼ 1 8g jbulk

( ð 1 pÞ 4

V X

) Qð j; g; p; pˆ Þ

j¼1

ð11Þ

ð12Þ

and ! 1 ðagÞ ðagÞ2 ðagÞ3 ag DðagÞu 15 þ e 4 3 6 6 !Z V 1 ðagÞ4 eak 2 ðagÞ : þ dk 2 12 k g

ð13Þ

The analytical result extends earlier results [7,9] and permits an efficient evaluation in the case where the degree of specular and diffusive scattering differs at the upper and lower boundary. The result (Eq. (13)) describes, in particular, the case when a thin (undoped) SiC transport channel is located below an oxide ( p + = 0) and on top of a doped SiC substrate ( p Y 1) or on a Si substrate (0 < p < 1, depending on the quality of the interface). Fig. 4 documents the significant phonon Knudsen effect caused by the interface scattering in two typical structures (insets) at two different temperatures. The figure shows the variation in the effective thermal conductivity j eff evaluated as the weighted average of the (interface limited) thermal conductivities describing the (finite) oxide, (finite) SiC and

640

E. Ziambaras, P. Hyldgaard / Materials Science and Engineering C 25 (2005) 635 – 640

finite Si-substrate layers. The figure documents that the Knudsen effect causes a very significant suppression of the thermal transport even up to hundreds of nanometers (micrometers) in the room liquid-nitrogen temperature cases. Fig. 4 further documents that calculations based on the traditional approach using Fourier law of heat conductions are inadequate due to the micron-scale phonon mean free path. The panels compare calculations with such a finiteelement type description (dotted curves) against the present phonon-based transport calculations assuming both diffusive (solid curves) and specular (dashed curves) scattering at the SiC/Si-substrate interface. We find that the traditional approach completely breaks down at lower temperatures and that moving to phonon-based calculations of thermal transport is essential for quantitative discussions of heat dissipation at room temperatures.

description of heat transport based on the Fourier law. We conclude that the introduction of multiple interfaces and/or continued reduction of the thickness of the substrate or the conduction channels have adverse effects on the overall device heat dissipation. The ongoing quest for miniaturization motivates a shift toward phonon-based calculations of the thermal transport in nanostructure devices.

Acknowledgment This work was supported by the Swedish National Graduate School in Material Science NFSM and by the Swedish Foundation for Strategic Research SSF through the consortium ATOMICS.

References 4. Conclusions In this paper we have documented significant suppressions of the thermal transport both across a SiC/metal or SiC/substrate interface and within the SiC layer between a top oxide and the substrate. For the room-temperature thermal conductance we find that it is the ratio of material sound velocities, rather than of the acoustic impedances, which should be adjusted to maximize the thermal transport. For the thermal transport in a layered structure we further documented that interface scattering causes a significant suppression for nanoscale (microscale) layer thicknesses at room (liquid-nitrogen) temperatures. Neither of these heattransport effects can be addressed within the traditional

[1] D.G. Cahill, W.K. Ford, K.E. Goodson, G. Mahan, A. Majumdar, H.J. Maris, R. Merlin, S.R. Phillpot, J. Appl. Phys. 93 (2003) 793. [2] P. Hyldgaard, G.D. Mahan, Phys. Rev., B 56 (1997) 10754. [3] P. Hyldgaard, cond-mat/0401315, Phys. Rev., B 69 (2004) 1933XX. [4] O. Madelung (Ed.), Landolt-Bornstein: Numerical Data and Functional Relationships in Science and Technology, New Series, Group III, vol. 17c, Springer, Berlin, 1982. [5] S. Pettersson, G.D. Mahan, Phys. Rev., B 42 (1990) 7386; R.J. Stoner, H.J. Maris, Phys. Rev., B 48 (1993) 16373. [6] J.M. Ziman, Electrons and Phonons, Oxford University Press, Oxford, 1960, p. 264. [7] P. Hyldgaard, G.D. Mahan, Thermal Conductivity, vol. 23, Technomic, Lancaster, PA, 1996, pp. 172 – 182. [8] K. Fuchs, Proc. Camb. Philos. Soc. 34 (1938) 100. [9] S.G. Walkauskas, D.A. Broido, K. Kempa, J. Appl. Phys. 85 (1999) 2579.

Copyright © 2021 COEK.INFO. All rights reserved.